Gallium(III) oxide is an inorganic compound and ultra-wide bandgap semiconductor with the formula Ga2O3. It is actively studied for applications in power electronics, phosphors, and gas sensing. The compound has several polymorphs, of which the monoclinic β-phase is the most stable. The β-phase’s bandgap of 4.7–4.9 eV and large-area, native substrates make it a promising competitor to GaN and SiC-based power electronics applications and solar-blind UV photodetectors. Ga2O3 exhibits reduced thermal conductivity and electron mobility by an order of magnitude compared to GaN and SiC, but is predicted to be significantly more cost-effective due to being the only wide-bandgap material capable of being grown from melt. β-Ga2O3 is thought to be radiation hard which makes it promising for military and space applications. Preparation Gallium trioxide is precipitated in hydrated form upon neutralization of acidic or basic solution of gallium salt. Also, it is formed on heating gallium in air or by thermally decomposing gallium nitrate at 200–250 ˚C. Crystalline Ga2O3 can occur in five polymorphs, α, β, γ, δ, and ε. Of these polymorphs β-Ga2O3 is the most thermodynamically stable phase at standard temperature and pressure while α-Ga2O3 is the most stable polymorph under high pressures. β-Ga2O3 Epitaxial thin films can be deposited heteroepitaxially on substrates such as sapphire, GaN, SiC, and Si, as well as homoepitaxially. For example, ALD on sapphire substrates at temperatures between 190 °C and 550 °C have been demonstrated. High quality β-Ga2O3 films have also been grown using techniques such as MBE, HVPE, and MOVPE. HVPE is preferred for vertical power semiconductor devices due to its fast growth rate. β-Ga2O3 epitaxial films grown by MOVPE exhibit higher electron mobilities and lower background carrier concentrations than those grown by other thin film growth techniques. Bulk substrates of β-Ga2O3 can be produced, which is one of the major advantages of this material system. Bulk substrates can be produced in multiple orientations and by multiple techniques. α-Ga2O3 can be obtained by heating β-Ga2O3 at 65 kbars and 1100 °C. It has a corundum structure. The hydrated form can be prepared by decomposing precipitated and "aged" gallium hydroxide at 500 °C. Epitaxial thin films of α-Ga2O3 deposited on c-plane (0001), m-plane (10-10), or a-plane (11-20) sapphire substrates have been demonstrated. γ-Ga2O3 is prepared by rapidly heating the hydroxide gel at 400–500 °C. A more crystalline form of this polymorph can be prepared directly from gallium metal by a solvothermal